During the construction of brides , dams or any other
structure where the foundation part of the structure is
most likely to lie underwater, we have to opt for
Construction in water poses many difficulties especially
in the places where there the depth is considerable.
During underwater construction our main objective is to
create dry and water free environment for working in such
a manner that the structural stability of the structure is not
Tremie method. Pump method. Toggle bags. Bags work.
It is a process in which the prepared concrete is
poured below the water surface by using suitable
A Tremie is a watertightpipe
Generally 250mm in dia.
Funnel shaped hopper at its upper end
and a loose plug at the bottom.
It is supported on a working platform
above water level.
Laying of concrete by using Tremie
Basic principle behind Method
of underwater concreting -
Method of underwater
method (inside view)
Specifications of concrete to be used in
Coarse Aggregate: Gravel of 3/4” (20mm) max. size. Use 50-55 %
of the total aggregate by weight.
Sand, 45-50% of the total aggregate by weight.
Cement: Type II ASTM (moderate heat of hydration), 600 lbs./yd3
Water/Cement Ratio: 0.42 (0.45 Maximum).
Water-Reducing Admixture (preferably it is also plasticizer): Do not
use super plasticizers.
Air-EntrainmentAdmixtures: To give 6% total air.
RetardingAdmixture: To increase setting time to 4-24 hours, as
Slump: 6 1/2" ± 1"
This mix will develop compressive strength in the range of 5,600 –
7,000 psi at 28 days.
Pumping concrete directly into its final
position, involving both horizontal and
vertical delivery of concrete.
Pumping concrete has the advantage of
operational efficiency with potential
savings of time and labour.
structures, the pump method should be
PUMP METHOD OF LAYING
• Toggle bags are ideal for
small amounts of concrete
• The bag is filled in the dry
with wet concrete
• Used for repair work.
• The concrete is squeezed
out by a diver.
• Bags are made of open
• Diver-handled bags are
usually of 10 to 20 litres
capacity but 1cub.m bags
can be placed using a crane.
Used only in special cases like repair works, etc.
Concrete spraying technology commonly known as guniting. when
concrete quality is good the structure concrete is impermeable.
Reduction in water cement ratio eliminates capillary pores so the
aim of spraying is homogeneous layer of concrete with reduced
w/c to discontinue the capillary pores.
In the early 1900’s, Carl Akeley, a famous hunter, naturalist and
professor, devised a novel method of making plaster models of large
animals for taxidermy work. He made a wire frame, and with a special
gun he devised, sprayed plaster onto the frame by means of compressed
Gunite can be defined as mortar conveyed through a hose
and pneumatically projected at a high velocity on the
There is not much difference between guniting and
shotcreting. Gunite was first used in the early 1900 and
this is mostly used for pneumatical application of mortar of
less thickness, whereas shotcrete is recent development on
the similar principal of guniting for achieving greater
thickness with small coarse aggregates.
Gunite has been used
since the early 1900’s
with excellent success.
There are two different
methods of spraying:
– Dry mix process spraying
– Wet mix process spraying
DRY MIX PROCESS
In this process, a mixture of cement and moist sand is
conveyed through the delivery hose to a nozzle where most of
the mixing water is added under pressure. This process
consists of the following steps:
a) The cement and moist sand are thoroughly mixed;
b) The cement-sand mixture is fed into a special mechanical
feeder or gun referred to as delivery equipment .
c) The mixture is forced into the delivery hose by a
d) The mixed material is carried in suspension by
compressed air through the delivery hose to a nozzle, which
is filled inside with a perforated manifold through which
water is introduced under pressure and intimately mixed
with the other ingredients; and
e) The mortar is jetted from the nozzle at high velocity on to
the surface to be shotcreted.
WET MIX PROCESS
In this process, all the ingredients including water are mixed
before they enter the delivery hose. It consists of the following
a) All the ingredients ( including mixing water) are thoroughly
b) The mortar or concrete is introduced into the chamber of the
c) The mixture is forced into the delivery hose and conveyed by
compressed air or other means to a nozzle;
d) Additional air is injected at the nozzle to increase the velocity
and improve the shooting pattern; and
e) The mortar or concrete is jetted from the nozzle at high velocity
on to the surface to be shotcreted.
Comparison of the dry and wet –
Dry-mix process Wet-mix process
Instantaneous control over
mixing water and consistency of
mix at the nozzle to meet
variable field conditions.
Better suited for placing mixes
aggregates, refractory materials
and shotcrete requiring early
Capable of being transported
Start and stop placement
characteristics are better with
minimal waste and greater
Capable of higher strengths
Mixing water is controlled at
the delivery equipment and
can be accurately measured.
Better assurance that the
mixing water is thoroughly
mixed with other ingredients
Less dusting and cement loss
accompanies the gunning
Normally has less rebound
resulting in less material
Capable of greater production
Properties of Gunite
•Properly applied gunite is a structurally adequate and durable material capable of
excellent bond with concrete, masonry, steel and other materials.
•The water-cement ratio for gunite in place normally falls within the range of 0.35
to 0.50 by mass which is somewhat lower than for most conventional concrete
• Most reported values for 28 days strength is in the range of 200 to 500kg/cm.
•The drying shrinkage generally falls within the range of 0.06 to 0.10 percent.
• The velocity will be about 90 to 120 m/s.
New structures: roofs ,walls, prestressed tanks, reservoir linings, canal lining,
swimming pools .tunnels, sewers and shafts.
coatings: over brick masonry, concrete, rock and steel.
encasement: of structural steel for fireproofing and reinforcing.
strengthening: of concrete slabs and concrete and masonry walls.
repair: of deteriorated concrete in structures such as reservoir
linings, dams, tunnels, shafts, elevators, waterfront
structures, and pipe. Repair of earthquake and fire damage
to masonry and concrete structures.
refractory linings: in stacks furnace walls and boilers.
USES OF GUNITE